Precursor polymorph determines the organic semiconductor ... ... Precursor polymorph determines the
Embed Size (px)
Text of Precursor polymorph determines the organic semiconductor ... ... Precursor polymorph determines the
aDipartimento di Chimica Industriale “Toso Montanari”, University of Bologna, Viale del Risorgimento 4, 40136, Bologna, Italy
bDipartimento di Chimica ‘‘G. Ciamician’’, University of Bologna, Via F. Selmi 2, 40126, Bologna, Italy
cInstitut de Ciència de Materials de Barcelona, ICMAB-CSIC, Campus de la UAB, 08193, Bellaterra, Spain
dDepartment of Chemical and Biological Physics, Weizmann Institute of Science, Rehovot 76100, Israel
Electronic Supplementary Material (ESI) for Journal of Materials Chemistry C. This journal is © The Royal Society of Chemistry 2021
Synthesis of N,N-Bis(tert-butyloxycarbonyl)-quinacridone (tBoc-QA)
Quinacridone (QA, 1.15 g, 3.68 mmol), di-tert-butyl dicarbonate (tBoc2O) (3.87 g, 17.7 mmol), 4-
dimetylaminopyridine (DMAP) (0.90 g, 7.37 mmol) were mixed in CH2Cl2 (184 mL) and reacted under
an inert atmosphere for 48 h at room temperature. The solvent was then removed at reduced
pressure and the crude product was purified by column chromatography (SiO2, toluene/ethyl
acetate 9:1). The resulting product was recrystallized several times from ethyl acetate to give 0.96
g (1.87 mmol) of a yellow solid (51% yield).
NMR and Mass spectroscopy
1H NMR spectra were recorded on a Varian Mercury Plus (400 MHz) spectrometer using
tetramethylsilane as a reference. Mass spectroscopy (electrospray ionization, ESI) spectra were
carried out on a Waters XEVO Q-TOF instrument.
1H NMR (400 MHz, CDCl3) δ 8.74 (s, 2H, HA), 8.41 (dd, J = 8.01, 1.56 Hz, 2H, HB), 7.84 (d, J = 8.79 Hz,
2H, HC), 7.72 (m, J = 8.49, 7.13, 1.56 Hz, 2H, HD), 7.38 (t, 7.52 Hz, 2H, HE), 1.77 (s, 18H, -CH3).
MS: m/z 513 [M]+; 457 [M-C4H8]+; 413 [M-C5H8O2]+; 357 [M-2(C4H8)]+; 313 [M-2(C5H8O2)]+.
Figure S 1 Upper panel: 1H NMR spectrum of tBoc-QA in CDCl3 (the singlet at 7.24 ppm is ascribable to CHCl3). Lower panel: mass spectrum (positive ions) of tBoc-QA.
X-ray single crystal structures of tBoc-QA polymorphs I and II.
Table S1. Crystal data and refinement details for crystalline tBoc-QA form I and form II.
Form I Form II
R1[on F0 2, I>2σ(I)] 0.0476 0.0583
wR2 (all data) 0.1124 0.1050
At ambient conditions, the latent pigment tBoc-QA may appear in two different polymorphic
modifications, named here form I and II. The former corresponds to the already known crystal
structure of this compound,1 and can be prepared by conventional recrystallization from ethyl
acetate of the as-synthesized material. The latter was identified in this work by lattice phonon
Raman microscopy and XRD on specimens obtained by drop-casting acetone solutions onto glass at
75°C and in films prepared by the BAMS method (see main text). tBoc-QA form I structure was redetermined in this work by single-crystal X-ray analysis. The crystal
is monoclinic with space group P21/n and cell parameters a = 14.149(1)Å, b = 6.5255(6)Å, c =
14.357(1)Å, β = 105.550(8)°. There are two centrosymmetric molecules per cell, with the
asymmetric unit consisting of half a molecule. The tert-butoxycarbonyl group bonded to the N-atom
is twisted by 54.3(2)° from the heterocyclic ring to which it is attached and the condensed ring
system is not perfectly planar, as the dihedral angle between two condensed rings is found to be≈
175°. No specific intermolecular interactions are present. Translationally equivalent molecules of tBoc-QA are arranged with the aromatic rings forming stacks in a face-to-face fashion.
The crystal structure of tBoc-QA form II was also determined by single-crystal X-ray analysis. The
unit cell is monoclinic with space group P21/c and cell parameters a = 23.791(3) Å, b = 6.1680(10) Å,
c = 19.031 Å, β = 112.076(18)°. There are four centrosymmetric molecules per cell, with the
asymmetric unit consisting of two half molecules, denoted as A and B. Each tBoc group is twisted
with respect to the corresponding heterocyclic ring by 64.5(5)° and 77.6(5)° for molecules A and B,
respectively. The condensed ring systems are, again, not perfectly planar, with a dihedral angle
between the central benzene ring and the neighboring ones of ≈ 175° and 177° for molecules A and
B, respectively. Form II structure features two distinct sets of face-to-face stacks generated by the
translation of the independent A and B molecules.
Figure S 2 Side and top views of the overlap among the molecules of tBoc-QA present in forms I and II showing the main differences in the orientation of the tBoc group with respect to the aromatic system. Form I in purple, form II in blue and orange for molecules A
and B, respectively. HCH atoms omitted for clarity.
Figure S 3 Crystal packing diagrams viewed along the b-axis for tBoc-QA form I (left) and form II (right). HCH atoms omitted for clarity.
Figure S 4 Comparison of the face-to-face stacking arrangements detected within crystalline tBoc-QA forma I and II. HCH atoms omitted for clarity.
Thermochemical cleavage of the tBoc protection group
Figure S 5 Optical photographs under polarized light of a crystal of tBoc-QA form I taken during the thermal deprotection process.
Figure S 6 a) Thermogram of a polycrystalline sample of tBoc-QA form I; DSC trace of a polycrystalline sample of tBoc-QA form I.
Figure S 7 IR spectra of tBoc-QA before (orange trace) and after (red trace) the thermochemical cleavage of the tBoc protection groups. In the inset the details of the N-H stretching region used to assess the reaction progression.
Raman characterization of tBoc-QA polymorphs
Figure S 8 Raman Spectra in the lattice phonon range (left) and in the 1400-1700 cm-1 intramolecular range (right) for tBoc-QA films obtained by the spin coating technique with solution of various solvents. In all cases the presence of the tBoc-QA crystal form I is
confirmed by the lattice phonon pattern.
Figure S9 shows the Raman spectra in the lattice phonon region for the crystallite obtained by drop
casting tBoc-QA acetone solutions on a glass substrate at RT (left) and at 75°C (right). The two
coloured traces correspond to the spectra of randomly oriented crystallites. The differences
between the spectral features of the patterns allow for the identification of the two different crystal
forms I and II. Such an identification id also supported by the Raman analysis in polarized light.
Spectra identified in the Figure with the PARPAR, PERPER and PARPER labels correspond to polarized
light measurements performed in backscattering geometry on single crystals oriented along their
extinction directions, as shown by the arrows in the Figure. For monoclinic systems like those under
study, such a direction is either parallel/perpendicular to the b crystal axis or lies in the ac crystal
plane, and such a knowledge is used to align the crystal axes with respect to the laboratory reference
frame. In both the measurement configurations labelled PARPAR and PERPER in the Figure, the
spectra are collected keeping incident and scattered light linearly polarized parallel to each other,
while the crystal has been rotated by 90°. In the spectra labelled as PARPER incident and scattered
light are crossed polarized.
Figure S 9 Raman spectra in the lattice phonon region of tBoc-QA crystallites obtained from the drop cast of acetone solutions at RT (left) and at 75°C (right) on a glass substrate. The optical images show the two different observed morphologies, and the arrows indicate the crystal extinction directions as detected in that area of the sample. The RT deposition is found to yield tBoc-QA form I; the 75°C yields form II. The asterisk marks a band of the substrate.
Following the symmetry Raman selection rules, and in agreement with symmetry properties of the
polarizability tensor which governs the intensity of the Raman signal, the polarized light Raman
measurements allow for the selective detection of vibrational modes of different symmetry. In this
work, in which they are used to discriminate more effectively between two crystalline forms, the
change in the relative peak intensities of the various measurement geometries allows for a better
definition of the spectral features both in the single crystals and in the films.
The red and black traces of Figure S10 correspond to the two typical Raman patterns detected in
the lattice phonon region when tBoc-QA films fabricated by the BAMS method are kept at a fixed
orientation with respect to the laboratory reference frame and are measured in parallel polarized
light, as explained in the main text of this work. In the Figure the spectra are compared to the
polarized Raman spectra collected on a single crystal.
Figure S 10 The two typical form II lattice phonon Raman patterns observed in the tBoc-QA films prepared by BAMS method compared to the polarized light spectra of form II single crystal (see also Figure S 9). The asterisk marks a band of the substrate.
DFT Calculations of QA and tBoc-QA normal vibrational modes
To aid the normal mode assignments for the bands detected in the vibrational spectra of QA and
tBoc-QA DFT simulations were performed. All calculations used GAUSSIAN 16 program package2.
The geometry optimization and energy calculations were carried out using B3LYP/6-311G++**
functional/basis-set and the frequencies computed at the harmonic level were scaled by the factor
given for this combination3. For the frequency range used as diagnostic for the thermal de-
protection, a comparison between simulated and experimental spectra is shown in Figure S10.
Tables S2,S3 report the calculated frequencies and the representations of the eigenvectors for the
selected modes of the two species. The isolated QA molecule possesses C2h symmetry, and the
normal modes classify as Ag, Bg, Au and Bu. All the in-plane Raman active modes belong to the total
symmetric representation Ag. The inversion centre (with the g/u character) is preserved in all the
crystal structures. The isolated tBoc-QA belongs to the Ci symmetry group and normal modes classify
as Ag, Au , with those belonging to the total symmetric representation Ag beeing Raman active. The
inversion centre is preserved in crystal form I; in crystal form II the molecule lies in a general position
but with a geometry only slightly different from the that of isolated molecule.
Figure S 11 Experimental and calculated Raman spectra in the energy range of the intramolecular vibrations used to monitor the thermal de-protection of the films.
Table S 2 Experimental and computed wavenumbers for the normal modes of QA in the interval 1400-1600 cm-1, with symmetry assignments and eigenvector graphical representations.
Exp frequency (cm1)
1437 Ag 1423
1482 Ag 1483
1517 Ag 1502
1567 Ag 1578
1598 Ag 1586
1631 Ag 1616
Table S 3 Experimental and computed wavenumbers for the normal modes of tBoc-QA in the interval 1400-1600 cm-1, with symmetry assignments and eigenvector graphical representations.
Exp frequency (cm1)
Symmetry Scaled DFT frequency
1. Mizuguchi, J. Di-tert-butyl 7, 14-dihydro-7, 14-dioxo-quino[2,3-b]acridine-5, 12-dicarboxylate. Acta Crystallogr. Sect. E 59, o474–o475 (2003).
2. Gaussian 16, Revision A.03, M. J. Frisch, G. W. Trucks, H. B. Schlegel, G. E. Scuseria, M. A. Robb, J. R. Cheeseman, G. Scalmani, V. Barone, G. A. Petersson, H. Nakatsuji, X. Li, M. Caricato, A. V. Marenich,J. Bloino, B. G. Janesko, R. Gomperts, B. Mennucci, H. P. Hratchian, J. V. Ortiz, A. F. Izmaylov, J. L. Sonnenberg, D. Williams-Young, F. Ding, F. Lipparini, F. Egidi, J. Goings, B. Peng, A. Petrone, T. Henderson, D. Ranasinghe, V. G. Zakrzewski, J. Gao, N. Rega, G. Zheng, W. Liang, M. Hada, M. Ehara, K. Toyota, R. Fukuda, J. Hasegawa, M. Ishida, T. Nakajima, Y. Honda, O. Kitao, H. Nakai,T. Vreven, K. Throssell, J. A. Montgomery, Jr., J. E. Peralta, F. Ogliaro, M. J. Bearpark, J. J. Heyd, E. N. Brothers, K. N. Kudin, V. N. Staroverov, T. A. Keith, R. Kobayashi, J. Normand, K. Raghavachari, A. P. Rendell, J. C. Burant, S. S. Iyengar, J. Tomasi, M. Cossi, J. M. Millam, M. Klene, C. Adamo, R. Cammi, J. W. Ochterski, R. L. Martin, K. Morokuma, O. Farkas, J. B. Foresman, and D. J. Fox, Gaussian, Inc., Wallingford CT, (2016.)
3. https://cccbdb.nist.gov/vsfx.asp; M. P. Andersson and P. Uvdal; New Scale Factors for Harmonic Vibrational Frequencies Using the B3LYP Density Functional Method with the Triple-ζ Basis Set 6- 311+G(d,p); J. Phys. Chem. A 2005, 109, 12, 2937–2941; 10.1021/jp045733a